#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:35:46 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179414 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/11/4331188.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4331188
loop_
_publ_author_name
'Leonid Unverfehrt'
'Markus Ströbele'
'H.-Jürgen Meyer'
_publ_section_title
;
 LaSr3F5(CN2)2: A Prototype Structure for Mixed-Valent Eu4F5(CN2)2
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              12925
_journal_page_last               12928
_journal_paper_doi               10.1021/ic302039q
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         'C2 F5 La N4 Sr3'
_chemical_formula_sum            'C2 F5 La N4 Sr3'
_chemical_formula_weight         576.83
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           121
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I -4 2'
_symmetry_space_group_name_H-M   'I -4 2 m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   8.086(2)
_cell_length_b                   8.086(2)
_cell_length_c                   6.580(2)
_cell_measurement_reflns_used    8000
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.07
_cell_measurement_theta_min      3.56
_cell_volume                     430.2(2)
_computing_cell_refinement       'STOE IPDS-Software'
_computing_data_collection       'STOE IPDS-Software'
_computing_data_reduction        'STOE IPDS-Software'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'STOE IPDS I'
_diffrn_measurement_method       Oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0449
_diffrn_reflns_av_sigmaI/netI    0.0168
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            2393
_diffrn_reflns_theta_full        26.07
_diffrn_reflns_theta_max         26.07
_diffrn_reflns_theta_min         3.56
_diffrn_standards_decay_%        0.0001
_exptl_absorpt_coefficient_mu    23.411
_exptl_absorpt_correction_T_max  0.1311
_exptl_absorpt_correction_T_min  0.0282
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'STOE X-Red/X-Shape'
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    4.453
_exptl_crystal_description       bloc
_exptl_crystal_F_000             512
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.688
_refine_diff_density_min         -0.748
_refine_diff_density_rms         0.186
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.02(4)
_refine_ls_extinction_coef       0.0096(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.290
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     20
_refine_ls_number_reflns         239
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.290
_refine_ls_R_factor_all          0.0203
_refine_ls_R_factor_gt           0.0201
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0345P)²+0.4375P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0557
_refine_ls_wR_factor_ref         0.0559
_reflns_number_gt                237
_reflns_number_total             239
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302039q_si_001.cif
_cod_data_source_block           LaSr3F5(CN2)2
_cod_database_code               4331188
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x, -y, -z'
'-x, -y, z'
'-x, y, -z'
'-y, -x, z'
'-y, x, -z'
'y, -x, -z'
'y, x, z'
'x+1/2, y+1/2, z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
La1 La 0.16267(4) 0.16267(4) 0.25557(7) 0.013 Uani 0.25 2 d SP 1
Sr1 Sr 0.16267(4) 0.16267(4) 0.25557(7) 0.013 Uani 0.75 2 d SP 2
N1 N 0.0000 0.6493(8) 0.0000 0.052(2) Uani 1 2 d S .
C1 C 0.0000 0.5000 0.0000 0.0200(16) Uani 1 4 d S .
F1 F 0.3661(4) 0.3661(4) 0.1325(6) 0.0194(7) Uani 1 2 d S .
F2 F 0.0000 0.0000 0.0000 0.0158(14) Uani 1 8 d S .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F1 La1 F1 116.74(13) . 11
F1 La1 F2 118.69(10) . .
F1 La1 F2 124.57(10) 11 .
F1 La1 F1 142.50(8) . 12_545
F1 La1 F1 67.25(14) 11 12_545
F2 La1 F1 69.41(8) . 12_545
F1 La1 F1 142.50(8) . 10_455
F1 La1 F1 67.25(14) 11 10_455
F2 La1 F1 69.41(8) . 10_455
F1 La1 F1 74.87(16) 12_545 10_455
F1 La1 N1 74.73(9) . 5_655
F1 La1 N1 130.04(5) 11 5_655
F2 La1 N1 67.10(11) . 5_655
F1 La1 N1 76.31(10) 12_545 5_655
F1 La1 N1 133.91(13) 10_455 5_655
F1 La1 N1 74.73(9) . 2_565
F1 La1 N1 130.04(5) 11 2_565
F2 La1 N1 67.10(11) . 2_565
F1 La1 N1 133.91(13) 12_545 2_565
F1 La1 N1 76.31(10) 10_455 2_565
N1 La1 N1 99.83(11) 5_655 2_565
F1 La1 La1 160.80(9) . 3
F1 La1 La1 82.45(10) 11 3
F2 La1 La1 42.115(15) . 3
F1 La1 La1 42.41(7) 12_545 3
F1 La1 La1 42.41(7) 10_455 3
N1 La1 La1 93.18(9) 5_655 3
N1 La1 La1 93.18(9) 2_565 3
F1 La1 La1 77.93(10) . 11
F1 La1 La1 38.81(10) 11 11
F2 La1 La1 163.378(18) . 11
F1 La1 La1 97.66(9) 12_545 11
F1 La1 La1 97.66(9) 10_455 11
N1 La1 La1 121.31(11) 5_655 11
N1 La1 La1 121.31(11) 2_565 11
La1 La1 La1 121.263(15) 3 11
F1 La1 La1 39.54(9) . 11_554
F1 La1 La1 156.29(10) 11 11_554
F2 La1 La1 79.15(2) . 11_554
F1 La1 La1 129.27(10) 12_545 11_554
F1 La1 La1 129.27(10) 10_455 11_554
N1 La1 La1 54.749(14) 5_655 11_554
N1 La1 La1 54.749(14) 2_565 11_554
La1 La1 La1 121.263(15) 3 11_554
La1 La1 La1 117.47(3) 11 11_554
F1 La1 La1 132.63(7) . 4_556
F1 La1 La1 34.29(6) 11 4_556
F2 La1 La1 100.78(2) . 4_556
F1 La1 La1 73.46(9) 12_545 4_556
F1 La1 La1 34.02(9) 10_455 4_556
N1 La1 La1 149.76(4) 5_655 4_556
N1 La1 La1 100.31(2) 2_565 4_556
La1 La1 La1 63.407(9) 3 4_556
La1 La1 La1 64.57(2) 11 4_556
La1 La1 La1 153.381(9) 11_554 4_556
F1 La1 La1 132.63(7) . 2_556
F1 La1 La1 34.29(6) 11 2_556
F2 La1 La1 100.78(2) . 2_556
F1 La1 La1 34.02(9) 12_545 2_556
F1 La1 La1 73.46(9) 10_455 2_556
N1 La1 La1 100.31(2) 5_655 2_556
N1 La1 La1 149.76(4) 2_565 2_556
La1 La1 La1 63.407(9) 3 2_556
La1 La1 La1 64.57(2) 11 2_556
La1 La1 La1 153.381(9) 11_554 2_556
La1 La1 La1 53.185(18) 4_556 2_556
C1 N1 Sr1 125.46(11) . 3_565
C1 N1 La1 125.46(11) . 3_565
Sr1 N1 La1 0.000(11) 3_565 3_565
C1 N1 La1 125.46(11) . 2_565
Sr1 N1 La1 109.1(2) 3_565 2_565
La1 N1 La1 109.1(2) 3_565 2_565
C1 N1 Sr1 125.46(11) . 2_565
Sr1 N1 Sr1 109.1(2) 3_565 2_565
La1 N1 Sr1 109.1(2) 3_565 2_565
La1 N1 Sr1 0.000(18) 2_565 2_565
C1 N1 Sr1 91.96(11) . 12
Sr1 N1 Sr1 94.96(8) 3_565 12
La1 N1 Sr1 94.96(8) 3_565 12
La1 N1 Sr1 82.75(6) 2_565 12
Sr1 N1 Sr1 82.75(6) 2_565 12
C1 N1 Sr1 91.96(11) . 9_454
Sr1 N1 Sr1 82.75(6) 3_565 9_454
La1 N1 Sr1 82.75(6) 3_565 9_454
La1 N1 Sr1 94.96(8) 2_565 9_454
Sr1 N1 Sr1 94.96(8) 2_565 9_454
Sr1 N1 Sr1 176.1(2) 12 9_454
N1 C1 N1 180.000(1) 2_565 .
La1 F1 Sr1 101.65(14) . 11_554
La1 F1 La1 101.65(14) . 11_554
Sr1 F1 La1 0.000(14) 11_554 11_554
La1 F1 Sr1 118.55(12) . 12
Sr1 F1 Sr1 111.69(12) 11_554 12
La1 F1 Sr1 111.69(12) 11_554 12
La1 F1 La1 118.55(12) . 12
Sr1 F1 La1 111.69(12) 11_554 12
La1 F1 La1 111.69(12) 11_554 12
Sr1 F1 La1 0.00(2) 12 12
La1 F1 Sr1 118.55(12) . 10
Sr1 F1 Sr1 111.69(12) 11_554 10
La1 F1 Sr1 111.69(12) 11_554 10
Sr1 F1 Sr1 95.17(14) 12 10
La1 F1 Sr1 95.17(14) 12 10
La1 F1 La1 118.55(12) . 10
Sr1 F1 La1 111.69(12) 11_554 10
La1 F1 La1 111.69(12) 11_554 10
Sr1 F1 La1 95.17(14) 12 10
La1 F1 La1 95.17(14) 12 10
Sr1 F1 La1 0.00(2) 10 10
La1 F2 Sr1 116.727(16) . 4
La1 F2 La1 116.727(16) . 2
Sr1 F2 La1 95.77(3) 4 2
La1 F2 Sr1 116.727(16) . 2
Sr1 F2 Sr1 95.77(3) 4 2
La1 F2 Sr1 0.000(11) 2 2
La1 F2 La1 116.727(16) . 4
Sr1 F2 La1 0.000(19) 4 4
La1 F2 La1 95.77(3) 2 4
Sr1 F2 La1 95.77(3) 2 4
La1 F2 La1 95.77(3) . 3
Sr1 F2 La1 116.727(16) 4 3
La1 F2 La1 116.727(16) 2 3
Sr1 F2 La1 116.727(16) 2 3
La1 F2 La1 116.727(16) 4 3
La1 F2 Sr1 95.77(3) . 3
Sr1 F2 Sr1 116.727(16) 4 3
La1 F2 Sr1 116.727(16) 2 3
Sr1 F2 Sr1 116.727(16) 2 3
La1 F2 Sr1 116.727(16) 4 3
La1 F2 Sr1 0.00(2) 3 3
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La1 F1 2.463(4) .
La1 F1 2.502(4) 11
La1 F2 2.5076(7) .
La1 F1 2.520(3) 12_545
La1 F1 2.520(3) 10_455
La1 N1 2.621(4) 5_655
La1 N1 2.621(4) 2_565
N1 C1 1.207(6) .
N1 Sr1 2.621(4) 3_565
N1 La1 2.621(4) 3_565
N1 La1 2.621(4) 2_565
N1 Sr1 2.621(4) 2_565
N1 Sr1 3.1684(8) 12
N1 Sr1 3.1684(8) 9_454
C1 N1 1.207(6) 2_565
F1 Sr1 2.502(4) 11_554
F1 La1 2.502(4) 11_554
F1 Sr1 2.520(3) 12
F1 La1 2.520(3) 12
F1 Sr1 2.520(3) 10
F1 La1 2.520(3) 10
F2 Sr1 2.5076(7) 4
F2 La1 2.5076(7) 2
F2 Sr1 2.5076(7) 2
F2 La1 2.5076(7) 4
F2 La1 2.5076(7) 3
F2 Sr1 2.5076(7) 3
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Sr1 N1 C1 N1 0(100) 3_565 2_565
La1 N1 C1 N1 0(100) 3_565 2_565
La1 N1 C1 N1 0(100) 2_565 2_565
Sr1 N1 C1 N1 0(100) 2_565 2_565
Sr1 N1 C1 N1 0(94) 12 2_565
Sr1 N1 C1 N1 0(100) 9_454 2_565
F1 La1 F1 Sr1 180.0 11 11_554
F2 La1 F1 Sr1 0.0 . 11_554
F1 La1 F1 Sr1 93.14(6) 12_545 11_554
F1 La1 F1 Sr1 -93.14(6) 10_455 11_554
N1 La1 F1 Sr1 52.47(9) 5_655 11_554
N1 La1 F1 Sr1 -52.47(9) 2_565 11_554
La1 La1 F1 Sr1 0.0 3 11_554
La1 La1 F1 Sr1 180.0 11 11_554
La1 La1 F1 Sr1 0.0 11_554 11_554
La1 La1 F1 Sr1 -142.52(6) 4_556 11_554
La1 La1 F1 Sr1 142.52(6) 2_556 11_554
F1 La1 F1 La1 180.0 11 11_554
F2 La1 F1 La1 0.0 . 11_554
F1 La1 F1 La1 93.14(6) 12_545 11_554
F1 La1 F1 La1 -93.14(6) 10_455 11_554
N1 La1 F1 La1 52.47(9) 5_655 11_554
N1 La1 F1 La1 -52.47(9) 2_565 11_554
La1 La1 F1 La1 0.0 3 11_554
La1 La1 F1 La1 180.0 11 11_554
La1 La1 F1 La1 -142.52(6) 4_556 11_554
La1 La1 F1 La1 142.52(6) 2_556 11_554
F1 La1 F1 Sr1 -57.19(13) 11 12
F2 La1 F1 Sr1 122.81(13) . 12
F1 La1 F1 Sr1 -144.06(16) 12_545 12
F1 La1 F1 Sr1 29.67(13) 10_455 12
N1 La1 F1 Sr1 175.28(17) 5_655 12
N1 La1 F1 Sr1 70.33(14) 2_565 12
La1 La1 F1 Sr1 122.81(13) 3 12
La1 La1 F1 Sr1 -57.19(13) 11 12
La1 La1 F1 Sr1 122.81(13) 11_554 12
La1 La1 F1 Sr1 -19.72(18) 4_556 12
La1 La1 F1 Sr1 -94.67(8) 2_556 12
F1 La1 F1 La1 -57.19(13) 11 12
F2 La1 F1 La1 122.81(13) . 12
F1 La1 F1 La1 -144.06(16) 12_545 12
F1 La1 F1 La1 29.67(13) 10_455 12
N1 La1 F1 La1 175.28(17) 5_655 12
N1 La1 F1 La1 70.33(14) 2_565 12
La1 La1 F1 La1 122.81(13) 3 12
La1 La1 F1 La1 -57.19(13) 11 12
La1 La1 F1 La1 122.81(13) 11_554 12
La1 La1 F1 La1 -19.72(18) 4_556 12
La1 La1 F1 La1 -94.67(8) 2_556 12
F1 La1 F1 Sr1 57.19(13) 11 10
F2 La1 F1 Sr1 -122.81(13) . 10
F1 La1 F1 Sr1 -29.67(13) 12_545 10
F1 La1 F1 Sr1 144.06(16) 10_455 10
N1 La1 F1 Sr1 -70.33(14) 5_655 10
N1 La1 F1 Sr1 -175.28(17) 2_565 10
La1 La1 F1 Sr1 -122.81(13) 3 10
La1 La1 F1 Sr1 57.19(13) 11 10
La1 La1 F1 Sr1 -122.81(13) 11_554 10
La1 La1 F1 Sr1 94.67(8) 4_556 10
La1 La1 F1 Sr1 19.72(18) 2_556 10
F1 La1 F1 La1 57.19(13) 11 10
F2 La1 F1 La1 -122.81(13) . 10
F1 La1 F1 La1 -29.67(13) 12_545 10
F1 La1 F1 La1 144.06(16) 10_455 10
N1 La1 F1 La1 -70.33(14) 5_655 10
N1 La1 F1 La1 -175.28(17) 2_565 10
La1 La1 F1 La1 -122.81(13) 3 10
La1 La1 F1 La1 57.19(13) 11 10
La1 La1 F1 La1 -122.81(13) 11_554 10
La1 La1 F1 La1 94.67(8) 4_556 10
La1 La1 F1 La1 19.72(18) 2_556 10
F1 La1 F2 Sr1 -56.153(7) . 4
F1 La1 F2 Sr1 123.847(7) 11 4
F1 La1 F2 Sr1 164.34(9) 12_545 4
F1 La1 F2 Sr1 83.36(9) 10_455 4
N1 La1 F2 Sr1 -112.306(15) 5_655 4
N1 La1 F2 Sr1 0.0 2_565 4
La1 La1 F2 Sr1 123.847(7) 3 4
La1 La1 F2 Sr1 123.847(8) 11 4
La1 La1 F2 Sr1 -56.153(7) 11_554 4
La1 La1 F2 Sr1 96.738(12) 4_556 4
La1 La1 F2 Sr1 150.956(9) 2_556 4
F1 La1 F2 La1 56.153(8) . 2
F1 La1 F2 La1 -123.847(7) 11 2
F1 La1 F2 La1 -83.36(9) 12_545 2
F1 La1 F2 La1 -164.34(9) 10_455 2
N1 La1 F2 La1 0.0 5_655 2
N1 La1 F2 La1 112.306(15) 2_565 2
La1 La1 F2 La1 -123.847(8) 3 2
La1 La1 F2 La1 -123.847(7) 11 2
La1 La1 F2 La1 56.153(7) 11_554 2
La1 La1 F2 La1 -150.956(9) 4_556 2
La1 La1 F2 La1 -96.738(12) 2_556 2
F1 La1 F2 Sr1 56.153(8) . 2
F1 La1 F2 Sr1 -123.847(7) 11 2
F1 La1 F2 Sr1 -83.36(9) 12_545 2
F1 La1 F2 Sr1 -164.34(9) 10_455 2
N1 La1 F2 Sr1 0.0 5_655 2
N1 La1 F2 Sr1 112.306(15) 2_565 2
La1 La1 F2 Sr1 -123.847(8) 3 2
La1 La1 F2 Sr1 -123.847(7) 11 2
La1 La1 F2 Sr1 56.153(7) 11_554 2
La1 La1 F2 Sr1 -150.956(9) 4_556 2
La1 La1 F2 Sr1 -96.738(12) 2_556 2
F1 La1 F2 La1 -56.153(7) . 4
F1 La1 F2 La1 123.847(7) 11 4
F1 La1 F2 La1 164.34(9) 12_545 4
F1 La1 F2 La1 83.36(9) 10_455 4
N1 La1 F2 La1 -112.306(15) 5_655 4
N1 La1 F2 La1 0.0 2_565 4
La1 La1 F2 La1 123.847(7) 3 4
La1 La1 F2 La1 123.847(8) 11 4
La1 La1 F2 La1 -56.153(7) 11_554 4
La1 La1 F2 La1 96.738(12) 4_556 4
La1 La1 F2 La1 150.956(9) 2_556 4
F1 La1 F2 La1 180.0 . 3
F1 La1 F2 La1 0.0 11 3
F1 La1 F2 La1 40.49(9) 12_545 3
F1 La1 F2 La1 -40.49(9) 10_455 3
N1 La1 F2 La1 123.847(8) 5_655 3
N1 La1 F2 La1 -123.847(8) 2_565 3
La1 La1 F2 La1 0.0 11 3
La1 La1 F2 La1 180.0 11_554 3
La1 La1 F2 La1 -27.109(8) 4_556 3
La1 La1 F2 La1 27.109(8) 2_556 3
F1 La1 F2 Sr1 180.0 . 3
F1 La1 F2 Sr1 0.0 11 3
F1 La1 F2 Sr1 40.49(9) 12_545 3
F1 La1 F2 Sr1 -40.49(9) 10_455 3
N1 La1 F2 Sr1 123.847(8) 5_655 3
N1 La1 F2 Sr1 -123.847(8) 2_565 3
La1 La1 F2 Sr1 0.0 3 3
La1 La1 F2 Sr1 0.0 11 3
La1 La1 F2 Sr1 180.0 11_554 3
La1 La1 F2 Sr1 -27.109(8) 4_556 3
La1 La1 F2 Sr1 27.109(8) 2_556 3
